#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/37/4303731.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4303731
loop_
_publ_author_name
'Tao Yang'
'Junliang Sun'
'Guobao Li'
'Yingxia Wang'
'Jeppe Christensen'
'Zhanbing He'
'Kirsten E. Christensen'
'Xiaodong Zou'
'Fuhui Liao'
'Jianhua Lin'
_publ_section_title
;
Fe5O5[B6O10(OH)3].nH2O: Wave-Layered Iron Borate and Frustrated
Antiferromagnetism
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              11209
_journal_page_last               11214
_journal_paper_doi               10.1021/ic9016867
_journal_volume                  48
_journal_year                    2009
_chemical_formula_sum            'B12 Fe10 H8 O37'
_chemical_formula_weight         1288.28
_space_group_IT_number           13
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 103.627(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   15.3013(4)
_cell_length_b                   11.8762(4)
_cell_length_c                   16.2894(5)
_cell_measurement_reflns_used    9937
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      36.5159
_cell_measurement_theta_min      3.6651
_cell_volume                     2876.80(15)
_computing_cell_refinement       'CrysAlys RED'
_computing_data_collection       'CrysAlys CCD'
_computing_data_reduction        'CrysAlys RED'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.994
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0389
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            35990
_diffrn_reflns_theta_full        25.03
_diffrn_reflns_theta_max         25.03
_diffrn_reflns_theta_min         3.71
_exptl_absorpt_coefficient_mu    5.027
_exptl_absorpt_correction_T_max  0.860
_exptl_absorpt_correction_T_min  0.562
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
CrysAlis RED, Oxford Diffraction Ltd.,
Version 1.171.32.15 (release 10-01-2008 CrysAlis171 .NET)
(compiled Jan 10 2008,16:37:18)
Analytical numeric absorption correction using a multifaceted crystal
            model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
;
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    2.974
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             2456
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.03
_refine_diff_density_max         1.840
_refine_diff_density_min         -1.133
_refine_diff_density_rms         0.260
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.035
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     226
_refine_ls_number_reflns         36235
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.035
_refine_ls_R_factor_all          0.1354
_refine_ls_R_factor_gt           0.0569
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0890P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1765
_refine_ls_wR_factor_ref         0.2189
_reflns_number_gt                4209
_reflns_number_total             5068
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic9016867_si_002_2.cif
_cod_data_source_block           FeB-Superlattice
_cod_original_sg_symbol_H-M      'P 2/c'
_cod_original_formula_sum        'H8 B12 Fe10 O37'
_cod_database_code               4303731
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Fe1A Fe 0.22014(7) 0.37533(7) 0.13151(4) 0.00908(9) Uani 1 1 d . . .
Fe1B Fe 0.02856(7) 0.37355(7) 0.36794(4) 0.00908(9) Uani 1 1 d . . .
Fe1C Fe 0.46949(7) 0.37654(7) 0.13272(4) 0.00908(9) Uani 1 1 d . . .
Fe1D Fe 0.27967(7) 0.37263(7) 0.36830(4) 0.00908(9) Uani 1 1 d . . .
Fe2A Fe 0.17264(7) 0.55042(7) 0.44214(4) 0.00895(10) Uani 1 1 d . . .
Fe2B Fe 0.57780(7) 0.55142(7) 0.05892(4) 0.00895(10) Uani 1 1 d . . .
Fe2C Fe 0.07682(7) 0.55864(7) 0.06113(4) 0.00895(10) Uani 1 1 d . . .
Fe2D Fe 0.32696(7) 0.56189(7) 0.06017(4) 0.00895(10) Uani 1 1 d . . .
Fe3A Fe 0.37509(5) 0.50894(7) 0.25190(4) 0.00818(10) Uani 1 1 d . . .
Fe3B Fe 0.12430(5) 0.50716(6) 0.24949(4) 0.00818(10) Uani 1 1 d . . .
B11 B 0.2071(4) 0.1175(6) 0.1217(3) 0.0078(5) Uiso 1 1 d . . .
B12 B 0.4513(4) 0.1212(6) 0.1292(4) 0.0078(5) Uiso 1 1 d . . .
B13 B 0.0259(7) 0.1159(9) 0.3724(5) 0.0396(15) Uiso 1 1 d . . .
B14 B 0.2996(6) 0.1229(9) 0.3713(5) 0.0396(15) Uiso 1 1 d . . .
B21 B 0.1841(5) 0.2054(5) -0.0168(3) 0.0078(5) Uiso 1 1 d . . .
B22 B 0.4267(5) 0.1985(6) -0.0185(3) 0.0078(5) Uiso 1 1 d . . .
B23 B 0.0373(5) 0.1989(9) 0.5129(5) 0.0329(13) Uiso 1 1 d . . .
B24 B 0.3510(5) 0.2057(8) 0.5082(5) 0.0329(13) Uiso 1 1 d . . .
B31 B 0.5964(4) 0.7496(6) 0.1662(3) 0.0078(5) Uiso 1 1 d . . .
B32 B 0.1505(5) 0.7609(6) 0.3276(3) 0.0078(5) Uiso 1 1 d . . .
B33 B 0.3840(5) 0.7512(9) 0.1861(5) 0.0388(15) Uiso 1 1 d . . .
B34 B 0.0771(5) 0.7486(9) 0.1699(5) 0.0388(15) Uiso 1 1 d D . .
O1A O 0.0000 0.4511(4) 0.2500 0.0077(4) Uiso 1 2 d S . .
O1B O 0.2510(2) 0.4597(3) 0.2513(2) 0.0077(4) Uiso 1 1 d . . .
O1C O 0.5000 0.4493(4) 0.2500 0.0077(4) Uiso 1 2 d S . .
O2A O 0.2020(3) 0.5183(3) 0.05507(19) 0.0072(3) Uiso 1 1 d . . .
O2B O 0.4551(3) 0.5234(3) 0.06036(18) 0.0072(3) Uiso 1 1 d . . .
O2C O 0.0443(3) 0.5189(3) 0.44026(18) 0.0072(3) Uiso 1 1 d . . .
O2D O 0.2960(3) 0.5120(3) 0.44668(19) 0.0072(3) Uiso 1 1 d . . .
O3A O 0.1529(3) 0.4131(3) 0.35471(18) 0.0075(3) Uiso 1 1 d . . .
O3B O 0.5954(3) 0.4145(3) 0.13825(19) 0.0075(3) Uiso 1 1 d . . .
O3C O 0.0979(3) 0.4141(3) 0.13608(19) 0.0075(3) Uiso 1 1 d . . .
O3D O 0.3445(3) 0.4162(3) 0.14463(18) 0.0075(3) Uiso 1 1 d . . .
O4A O 0.6104(3) 0.6417(3) 0.1664(2) 0.0110(3) Uiso 1 1 d . . .
O4B O 0.1459(3) 0.6376(3) 0.3393(2) 0.0110(3) Uiso 1 1 d . . .
O4C O 0.3608(3) 0.6409(3) 0.1662(2) 0.0110(3) Uiso 1 1 d . . .
O4D O 0.1101(3) 0.6368(3) 0.1718(2) 0.0110(3) Uiso 1 1 d D . .
O5A O 0.1859(3) 0.3069(3) 0.0129(2) 0.0116(3) Uiso 1 1 d . . .
O5B O 0.4303(3) 0.3134(3) 0.0103(2) 0.0116(3) Uiso 1 1 d . . .
O5C O 0.0630(3) 0.3104(3) 0.4879(2) 0.0116(3) Uiso 1 1 d . . .
O5D O 0.3154(3) 0.3021(3) 0.4859(2) 0.0116(3) Uiso 1 1 d . . .
O6A O 0.2275(3) 0.2115(3) 0.1689(2) 0.0145(3) Uiso 1 1 d . . .
O6B O 0.0230(3) 0.2168(3) 0.3257(2) 0.0145(3) Uiso 1 1 d . . .
O6C O 0.4730(3) 0.2192(3) 0.1707(2) 0.0145(3) Uiso 1 1 d . . .
O6D O 0.2756(3) 0.2151(3) 0.3278(2) 0.0145(3) Uiso 1 1 d . . .
O7A O 0.2319(4) 0.0118(5) 0.1585(3) 0.0530(14) Uiso 1 1 d . . .
O7B O -0.0008(3) 0.0218(5) 0.3343(3) 0.0395(14) Uiso 1 1 d . . .
O7C O 0.4632(3) 0.0167(5) 0.1673(3) 0.0396(14) Uiso 1 1 d . . .
O7D O 0.3242(6) 0.0322(9) 0.3255(5) 0.0309(15) Uiso 0.50 1 d P . .
O7E O 0.2286(6) 0.0214(9) 0.3219(5) 0.0309(15) Uiso 0.50 1 d P . .
O8A O 0.2014(3) 0.1135(3) 0.0385(2) 0.0141(6) Uiso 1 1 d . . .
O8B O 0.4253(2) 0.1160(4) 0.0389(2) 0.0141(6) Uiso 1 1 d . . .
O8C O 0.0287(4) 0.1169(6) 0.4634(3) 0.067(2) Uiso 1 1 d . . .
O8D O 0.3311(4) 0.1153(5) 0.4573(3) 0.0591(17) Uiso 1 1 d . . .
O9A O 0.6013(2) 0.8053(3) 0.2456(2) 0.0182(9) Uiso 1 1 d . . .
O9B O 0.1259(3) 0.8041(3) 0.2538(2) 0.0241(9) Uiso 1 1 d D . .
O10A O 0.1726(2) 0.1792(3) -0.10060(19) 0.0116(5) Uiso 1 1 d . . .
O10B O 0.3952(2) 0.1768(3) -0.1020(2) 0.0116(5) Uiso 1 1 d . . .
O10C O 0.0208(4) 0.1884(7) 0.6035(4) 0.087(2) Uiso 1 1 d . . .
O10D O 0.3898(4) 0.8142(6) 0.1047(3) 0.0631(17) Uiso 1 1 d . . .
OW1A O 0.2256(4) 0.8124(6) 0.0707(4) 0.0200(14) Uiso 0.592(6) 1 d P . .
OW1B O 0.1991(6) 0.7934(9) 0.1314(6) 0.0200(14) Uiso 0.408(6) 1 d P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3D Fe1A O3C 150.43(15) . . ?
O3D Fe1A O6A 102.98(18) . . ?
O3C Fe1A O6A 101.60(18) . . ?
O3D Fe1A O5A 103.36(17) . . ?
O3C Fe1A O5A 95.50(16) . . ?
O6A Fe1A O5A 83.51(14) . . ?
O3D Fe1A O2A 81.36(17) . . ?
O3C Fe1A O2A 80.56(17) . . ?
O6A Fe1A O2A 161.46(13) . . ?
O5A Fe1A O2A 77.95(14) . . ?
O3D Fe1A O1B 77.38(14) . . ?
O3C Fe1A O1B 82.05(14) . . ?
O6A Fe1A O1B 100.92(13) . . ?
O5A Fe1A O1B 175.27(15) . . ?
O2A Fe1A O1B 97.62(13) . . ?
O6B Fe1B O3C 104.82(18) . 2 ?
O6B Fe1B O3A 98.39(18) . . ?
O3C Fe1B O3A 151.35(15) 2 . ?
O6B Fe1B O5C 88.16(15) . . ?
O3C Fe1B O5C 98.67(17) 2 . ?
O3A Fe1B O5C 98.63(16) . . ?
O6B Fe1B O2C 166.17(14) . . ?
O3C Fe1B O2C 78.32(16) 2 . ?
O3A Fe1B O2C 83.16(16) . . ?
O5C Fe1B O2C 78.03(15) . . ?
O6B Fe1B O1A 96.48(16) . . ?
O3C Fe1B O1A 82.57(10) 2 . ?
O3A Fe1B O1A 78.28(10) . . ?
O5C Fe1B O1A 174.74(17) . . ?
O2C Fe1B O1A 97.29(16) . . ?
O3B Fe1C O6C 104.51(18) . . ?
O3B Fe1C O3D 152.03(15) . . ?
O6C Fe1C O3D 98.50(17) . . ?
O3B Fe1C O1C 81.63(10) . . ?
O6C Fe1C O1C 97.13(16) . . ?
O3D Fe1C O1C 79.92(10) . . ?
O3B Fe1C O5B 100.67(15) . . ?
O6C Fe1C O5B 86.52(15) . . ?
O3D Fe1C O5B 96.34(15) . . ?
O1C Fe1C O5B 175.10(16) . . ?
O3B Fe1C O2B 78.78(16) . . ?
O6C Fe1C O2B 164.52(14) . . ?
O3D Fe1C O2B 83.28(16) . . ?
O1C Fe1C O2B 98.32(16) . . ?
O5B Fe1C O2B 78.00(14) . . ?
O3A Fe1D O6D 104.00(18) . . ?
O3A Fe1D O3B 149.90(14) . 2_655 ?
O6D Fe1D O3B 99.90(18) . 2_655 ?
O3A Fe1D O5D 104.23(17) . . ?
O6D Fe1D O5D 84.58(15) . . ?
O3B Fe1D O5D 95.94(16) 2_655 . ?
O3A Fe1D O2D 81.12(16) . . ?
O6D Fe1D O2D 162.03(14) . . ?
O3B Fe1D O2D 81.76(17) 2_655 . ?
O5D Fe1D O2D 77.45(14) . . ?
O3A Fe1D O1B 77.81(14) . . ?
O6D Fe1D O1B 100.24(13) . . ?
O3B Fe1D O1B 80.17(14) 2_655 . ?
O5D Fe1D O1B 174.22(15) . . ?
O2D Fe1D O1B 97.68(13) . . ?
O2D Fe2A O4B 99.55(19) . . ?
O2D Fe2A O2A 81.93(16) . 4_566 ?
O4B Fe2A O2A 172.10(16) . 4_566 ?
O2D Fe2A O2C 155.41(15) . . ?
O4B Fe2A O2C 94.64(18) . . ?
O2A Fe2A O2C 86.77(17) 4_566 . ?
O2D Fe2A O5A 102.11(17) . 4_566 ?
O4B Fe2A O5A 91.02(15) . 4_566 ?
O2A Fe2A O5A 81.08(14) 4_566 4_566 ?
O2C Fe2A O5A 97.58(18) . 4_566 ?
O2D Fe2A O3A 80.08(16) . . ?
O4B Fe2A O3A 82.13(14) . . ?
O2A Fe2A O3A 105.77(14) 4_566 . ?
O2C Fe2A O3A 82.11(17) . . ?
O5A Fe2A O3A 173.09(14) 4_566 . ?
O2B Fe2B O5B 102.81(18) . 3_665 ?
O2B Fe2B O2D 156.42(16) . 2_655 ?
O5B Fe2B O2D 95.54(17) 3_665 2_655 ?
O2B Fe2B O4A 97.17(17) . . ?
O5B Fe2B O4A 91.91(15) 3_665 . ?
O2D Fe2B O4A 96.88(16) 2_655 . ?
O2B Fe2B O3B 80.67(17) . . ?
O5B Fe2B O3B 175.38(17) 3_665 . ?
O2D Fe2B O3B 81.91(16) 2_655 . ?
O4A Fe2B O3B 84.60(14) . . ?
O2B Fe2B O2B 85.13(17) . 3_665 ?
O5B Fe2B O2B 80.99(15) 3_665 3_665 ?
O2D Fe2B O2B 83.23(16) 2_655 3_665 ?
O4A Fe2B O2B 172.87(16) . 3_665 ?
O3B Fe2B O2B 102.46(15) . 3_665 ?
O2B Fe2B Fe2B 44.87(10) . 3_665 ?
O5B Fe2B Fe2B 91.89(12) 3_665 3_665 ?
O2D Fe2B Fe2B 120.73(11) 2_655 3_665 ?
O4A Fe2B Fe2B 141.59(15) . 3_665 ?
O3B Fe2B Fe2B 92.73(11) . 3_665 ?
O2B Fe2B Fe2B 40.26(13) 3_665 3_665 ?
O2C Fe2C O5C 103.07(19) 2 4_565 ?
O2C Fe2C O4D 99.61(17) 2 . ?
O5C Fe2C O4D 98.69(15) 4_565 . ?
O2C Fe2C O2A 151.60(15) 2 . ?
O5C Fe2C O2A 97.38(18) 4_565 . ?
O4D Fe2C O2A 96.50(16) . . ?
O2C Fe2C O3C 79.60(17) 2 . ?
O5C Fe2C O3C 176.35(19) 4_565 . ?
O4D Fe2C O3C 83.21(14) . . ?
O2A Fe2C O3C 79.27(16) . . ?
O2C Fe2C O2C 82.34(17) 2 4_565 ?
O5C Fe2C O2C 79.05(15) 4_565 4_565 ?
O4D Fe2C O2C 177.33(17) . 4_565 ?
O2A Fe2C O2C 82.44(16) . 4_565 ?
O3C Fe2C O2C 98.98(14) . 4_565 ?
O4C Fe2D O2A 102.71(17) . . ?
O4C Fe2D O2D 176.12(17) . 4_565 ?
O2A Fe2D O2D 80.14(16) . 4_565 ?
O4C Fe2D O5D 96.64(15) . 4_565 ?
O2A Fe2D O5D 103.94(17) . 4_565 ?
O2D Fe2D O5D 80.04(14) 4_565 4_565 ?
O4C Fe2D O2B 93.04(17) . . ?
O2A Fe2D O2B 151.49(15) . . ?
O2D Fe2D O2B 85.45(16) 4_565 . ?
O5D Fe2D O2B 97.55(17) 4_565 . ?
O4C Fe2D O3D 81.61(14) . . ?
O2A Fe2D O3D 78.02(16) . . ?
O2D Fe2D O3D 101.65(14) 4_565 . ?
O5D Fe2D O3D 177.65(16) 4_565 . ?
O2B Fe2D O3D 81.02(16) . . ?
O1B Fe3A O3D 79.04(16) . . ?
O1B Fe3A O4A 100.80(16) . 2_655 ?
O3D Fe3A O4A 161.83(15) . 2_655 ?
O1B Fe3A O1C 142.61(14) . . ?
O3D Fe3A O1C 79.94(14) . . ?
O4A Fe3A O1C 108.59(16) 2_655 . ?
O1B Fe3A O3B 81.84(16) . 2_655 ?
O3D Fe3A O3B 114.24(14) . 2_655 ?
O4A Fe3A O3B 83.51(14) 2_655 2_655 ?
O1C Fe3A O3B 79.11(14) . 2_655 ?
O1B Fe3A O4C 105.69(16) . . ?
O3D Fe3A O4C 82.19(14) . . ?
O4A Fe3A O4C 80.38(14) 2_655 . ?
O1C Fe3A O4C 101.65(16) . . ?
O3B Fe3A O4C 163.23(15) 2_655 . ?
O4D Fe3B O3A 162.14(15) . . ?
O4D Fe3B O1B 100.87(17) . . ?
O3A Fe3B O1B 79.37(17) . . ?
O4D Fe3B O1A 107.38(17) . . ?
O3A Fe3B O1A 80.16(15) . . ?
O1B Fe3B O1A 144.46(15) . . ?
O4D Fe3B O4B 81.16(14) . . ?
O3A Fe3B O4B 81.32(14) . . ?
O1B Fe3B O4B 101.70(16) . . ?
O1A Fe3B O4B 103.54(17) . . ?
O4D Fe3B O3C 82.97(14) . . ?
O3A Fe3B O3C 114.52(14) . . ?
O1B Fe3B O3C 81.45(15) . . ?
O1A Fe3B O3C 81.07(14) . . ?
O4B Fe3B O3C 164.14(14) . . ?
O8A B11 O6A 123.9(5) . . ?
O8A B11 O7A 110.3(5) . . ?
O6A B11 O7A 119.6(4) . . ?
O6C B12 O7C 124.1(5) . . ?
O6C B12 O8B 121.9(5) . . ?
O7C B12 O8B 113.5(5) . . ?
O7B B13 O6B 120.3(7) . . ?
O7B B13 O8C 114.8(8) . . ?
O6B B13 O8C 121.7(7) . . ?
O6D B14 O8D 126.5(8) . . ?
O6D B14 O7D 115.3(7) . . ?
O8D B14 O7D 114.6(8) . . ?
O6D B14 O7E 105.7(6) . . ?
O8D B14 O7E 117.9(7) . . ?
O7D B14 O7E 55.0(5) . . ?
O5A B21 O10A 124.8(5) . . ?
O5A B21 O8A 120.0(4) . . ?
O10A B21 O8A 115.1(5) . . ?
O10B B22 O8B 119.6(5) . . ?
O10B B22 O5B 119.0(5) . . ?
O8B B22 O5B 117.7(4) . . ?
O8C B23 O5C 121.3(7) . . ?
O8C B23 O10C 122.1(8) . . ?
O5C B23 O10C 116.6(7) . . ?
O5D B24 O8D 121.2(6) . . ?
O5D B24 O10D 117.0(7) . 4_566 ?
O8D B24 O10D 118.4(7) . 4_566 ?
O4A B31 O10B 125.2(5) . 3_665 ?
O4A B31 O9A 118.6(5) . . ?
O10B B31 O9A 113.1(5) 3_665 . ?
O9B B32 O10A 124.4(6) . 4_566 ?
O9B B32 O4B 120.3(5) . . ?
O10A B32 O4B 114.9(4) 4_566 . ?
O9A B33 O4C 132.6(8) 2_655 . ?
O9A B33 O10D 118.5(8) 2_655 . ?
O4C B33 O10D 108.9(6) . . ?
O4D B34 O10C 131.0(7) . 4_565 ?
O4D B34 O9B 106.6(6) . . ?
O10C B34 O9B 121.8(8) 4_565 . ?
Fe3B O1A Fe3B 141.5(3) . 2 ?
Fe3B O1A Fe1B 97.78(4) . 2 ?
Fe3B O1A Fe1B 99.01(4) 2 2 ?
Fe3B O1A Fe1B 99.01(4) . . ?
Fe3B O1A Fe1B 97.78(4) 2 . ?
Fe1B O1A Fe1B 127.5(3) 2 . ?
Fe3A O1B Fe3B 146.62(18) . . ?
Fe3A O1B Fe1D 98.28(14) . . ?
Fe3B O1B Fe1D 98.33(17) . . ?
Fe3A O1B Fe1A 98.43(17) . . ?
Fe3B O1B Fe1A 96.47(13) . . ?
Fe1D O1B Fe1A 122.95(16) . . ?
Fe3A O1C Fe3A 139.5(3) . 2_655 ?
Fe3A O1C Fe1C 98.73(4) . . ?
Fe3A O1C Fe1C 98.07(4) 2_655 . ?
Fe3A O1C Fe1C 98.07(4) . 2_655 ?
Fe3A O1C Fe1C 98.73(4) 2_655 2_655 ?
Fe1C O1C Fe1C 130.1(3) . 2_655 ?
Fe2D O2A Fe2A 98.90(19) . 4_565 ?
Fe2D O2A Fe2C 150.4(2) . . ?
Fe2A O2A Fe2C 97.77(17) 4_565 . ?
Fe2D O2A Fe1A 101.43(18) . . ?
Fe2A O2A Fe1A 100.92(16) 4_565 . ?
Fe2C O2A Fe1A 99.19(18) . . ?
Fe2B O2B Fe2D 156.8(2) . . ?
Fe2B O2B Fe1C 100.32(18) . . ?
Fe2D O2B Fe1C 99.43(18) . . ?
Fe2B O2B Fe2B 94.87(17) . 3_665 ?
Fe2D O2B Fe2B 94.25(16) . 3_665 ?
Fe1C O2B Fe2B 98.06(17) . 3_665 ?
Fe2C O2C Fe2A 154.8(2) 2 . ?
Fe2C O2C Fe1B 102.54(18) 2 . ?
Fe2A O2C Fe1B 98.47(18) . . ?
Fe2C O2C Fe2C 97.66(17) 2 4_566 ?
Fe2A O2C Fe2C 92.99(15) . 4_566 ?
Fe1B O2C Fe2C 97.84(17) . 4_566 ?
Fe2A O2D Fe2D 99.00(19) . 4_566 ?
Fe2A O2D Fe2B 152.4(2) . 2_655 ?
Fe2D O2D Fe2B 97.06(17) 4_566 2_655 ?
Fe2A O2D Fe1D 101.05(17) . . ?
Fe2D O2D Fe1D 100.81(16) 4_566 . ?
Fe2B O2D Fe1D 97.80(18) 2_655 . ?
Fe1D O3A Fe3B 104.14(19) . . ?
Fe1D O3A Fe1B 149.7(2) . . ?
Fe3B O3A Fe1B 101.48(17) . . ?
Fe1D O3A Fe2A 97.54(16) . . ?
Fe3B O3A Fe2A 96.46(16) . . ?
Fe1B O3A Fe2A 95.44(17) . . ?
Fe1C O3B Fe1D 151.8(2) . 2_655 ?
Fe1C O3B Fe2B 99.87(17) . . ?
Fe1D O3B Fe2B 98.52(18) 2_655 . ?
Fe1C O3B Fe3A 100.16(18) . 2_655 ?
Fe1D O3B Fe3A 99.44(16) 2_655 2_655 ?
Fe2B O3B Fe3A 94.84(16) . 2_655 ?
Fe1A O3C Fe1B 151.9(2) . 2 ?
Fe1A O3C Fe2C 100.97(19) . . ?
Fe1B O3C Fe2C 99.52(17) 2 . ?
Fe1A O3C Fe3B 99.82(16) . . ?
Fe1B O3C Fe3B 98.06(17) 2 . ?
Fe2C O3C Fe3B 93.04(15) . . ?
Fe1A O3D Fe1C 149.5(2) . . ?
Fe1A O3D Fe3A 104.72(19) . . ?
Fe1C O3D Fe3A 100.27(17) . . ?
Fe1A O3D Fe2D 99.08(17) . . ?
Fe1C O3D Fe2D 95.91(17) . . ?
Fe3A O3D Fe2D 94.71(16) . . ?
B31 O4A Fe2B 121.1(3) . . ?
B31 O4A Fe3A 139.1(4) . 2_655 ?
Fe2B O4A Fe3A 97.00(17) . 2_655 ?
B32 O4B Fe2A 129.5(3) . . ?
B32 O4B Fe3B 130.1(3) . . ?
Fe2A O4B Fe3B 100.09(17) . . ?
B33 O4C Fe2D 132.4(4) . . ?
B33 O4C Fe3A 125.5(4) . . ?
Fe2D O4C Fe3A 101.43(18) . . ?
B34 O4D Fe3B 136.9(4) . . ?
B34 O4D Fe2C 113.8(4) . . ?
Fe3B O4D Fe2C 100.58(17) . . ?
B21 O5A Fe2A 124.9(3) . 4_565 ?
B21 O5A Fe1A 134.4(3) . . ?
Fe2A O5A Fe1A 100.00(17) 4_565 . ?
B22 O5B Fe2B 126.8(3) . 3_665 ?
B22 O5B Fe1C 129.4(3) . . ?
Fe2B O5B Fe1C 102.82(18) 3_665 . ?
B23 O5C Fe2C 123.5(4) . 4_566 ?
B23 O5C Fe1B 124.8(4) . . ?
Fe2C O5C Fe1B 105.07(19) 4_566 . ?
B24 O5D Fe2D 125.3(4) . 4_566 ?
B24 O5D Fe1D 129.2(5) . . ?
Fe2D O5D Fe1D 101.65(18) 4_566 . ?
B11 O6A Fe1A 129.1(3) . . ?
B13 O6B Fe1B 128.0(4) . . ?
B12 O6C Fe1C 132.7(3) . . ?
B14 O6D Fe1D 128.8(4) . . ?
B14 O7D O7E 72.5(7) . . ?
O7D O7E B14 52.5(6) . . ?
B11 O8A B21 125.5(5) . . ?
B22 O8B B12 129.2(5) . . ?
B23 O8C B13 128.9(8) . . ?
B24 O8D B14 123.3(7) . . ?
B33 O9A B31 121.4(6) 2_655 . ?
B32 O9B B34 129.4(5) . . ?
B32 O10A B21 134.0(5) 4_565 . ?
B22 O10B B31 124.1(5) . 3_665 ?
B34 O10C B23 118.2(7) 4_566 . ?
B33 O10D B24 135.0(6) . 4_565 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Fe1A O3D 1.927(4) . ?
Fe1A O3C 1.944(4) . ?
Fe1A O6A 2.034(4) . ?
Fe1A O5A 2.047(3) . ?
Fe1A O2A 2.085(4) . ?
Fe1A O1B 2.146(4) . ?
Fe1B O6B 1.980(4) . ?
Fe1B O3C 1.981(4) 2 ?
Fe1B O3A 2.020(5) . ?
Fe1B O5C 2.043(3) . ?
Fe1B O2C 2.072(4) . ?
Fe1B O1A 2.082(2) . ?
Fe1C O3B 1.960(5) . ?
Fe1C O6C 1.965(4) . ?
Fe1C O3D 2.023(5) . ?
Fe1C O1C 2.048(2) . ?
Fe1C O5B 2.082(4) . ?
Fe1C O2B 2.087(4) . ?
Fe1D O3A 1.959(5) . ?
Fe1D O6D 1.980(4) . ?
Fe1D O3B 2.003(5) 2_655 ?
Fe1D O5D 2.044(3) . ?
Fe1D O2D 2.069(3) . ?
Fe1D O1B 2.121(4) . ?
Fe2A O2D 1.926(5) . ?
Fe2A O4B 1.930(3) . ?
Fe2A O2A 1.965(3) 4_566 ?
Fe2A O2C 1.993(5) . ?
Fe2A O5A 2.032(4) 4_566 ?
Fe2A O3A 2.139(4) . ?
Fe2B O2B 1.912(5) . ?
Fe2B O5B 1.950(4) 3_665 ?
Fe2B O2D 2.011(5) 2_655 ?
Fe2B O4A 2.013(3) . ?
Fe2B O3B 2.055(4) . ?
Fe2B O2B 2.087(3) 3_665 ?
Fe2B Fe2B 2.9481(18) 3_665 ?
Fe2C O2C 1.907(5) 2 ?
Fe2C O5C 1.941(4) 4_565 ?
Fe2C O4D 1.985(3) . ?
Fe2C O2A 1.999(5) . ?
Fe2C O3C 2.087(4) . ?
Fe2C O2C 2.124(3) 4_565 ?
Fe2D O4C 1.927(4) . ?
Fe2D O2A 1.963(5) . ?
Fe2D O2D 2.000(3) 4_565 ?
Fe2D O5D 2.001(4) 4_565 ?
Fe2D O2B 2.013(5) . ?
Fe2D O3D 2.187(4) . ?
Fe3A O1B 1.985(4) . ?
Fe3A O3D 2.024(3) . ?
Fe3A O4A 2.042(4) 2_655 ?
Fe3A O1C 2.0453(19) . ?
Fe3A O3B 2.070(3) 2_655 ?
Fe3A O4C 2.076(4) . ?
Fe3B O4D 1.972(4) . ?
Fe3B O3A 2.006(3) . ?
Fe3B O1B 2.012(4) . ?
Fe3B O1A 2.0169(19) . ?
Fe3B O4B 2.102(4) . ?
Fe3B O3C 2.108(3) . ?
B11 O8A 1.339(6) . ?
B11 O6A 1.349(7) . ?
B11 O7A 1.405(8) . ?
B12 O6C 1.348(7) . ?
B12 O7C 1.380(8) . ?
B12 O8B 1.432(6) . ?
B13 O7B 1.298(10) . ?
B13 O6B 1.414(10) . ?
B13 O8C 1.472(10) . ?
B14 O6D 1.309(10) . ?
B14 O8D 1.372(9) . ?
B14 O7D 1.410(12) . ?
B14 O7E 1.695(13) . ?
B21 O5A 1.297(7) . ?
B21 O10A 1.370(6) . ?
B21 O8A 1.400(7) . ?
B22 O10B 1.355(6) . ?
B22 O8B 1.358(7) . ?
B22 O5B 1.440(7) . ?
B23 O8C 1.251(10) . ?
B23 O5C 1.466(10) . ?
B23 O10C 1.560(10) . ?
B24 O5D 1.283(10) . ?
B24 O8D 1.347(10) . ?
B24 O10D 1.562(9) 4_566 ?
B31 O4A 1.299(7) . ?
B31 O10B 1.393(7) 3_665 ?
B31 O9A 1.438(7) . ?
B32 O9B 1.279(6) . ?
B32 O10A 1.343(6) 4_566 ?
B32 O4B 1.481(7) . ?
B33 O9A 1.259(9) 2_655 ?
B33 O4C 1.375(11) . ?
B33 O10D 1.543(11) . ?
B34 O4D 1.418(11) . ?
B34 O10C 1.426(10) 4_565 ?
B34 O9B 1.542(9) . ?
O1A Fe3B 2.0169(19) 2 ?
O1A Fe1B 2.082(2) 2 ?
O1C Fe3A 2.0453(19) 2_655 ?
O1C Fe1C 2.048(2) 2_655 ?
O2A Fe2A 1.965(3) 4_565 ?
O2B Fe2B 2.087(3) 3_665 ?
O2C Fe2C 1.907(5) 2 ?
O2C Fe2C 2.124(3) 4_566 ?
O2D Fe2D 2.000(3) 4_566 ?
O2D Fe2B 2.011(5) 2_655 ?
O3B Fe1D 2.003(5) 2_655 ?
O3B Fe3A 2.070(3) 2_655 ?
O3C Fe1B 1.981(4) 2 ?
O4A Fe3A 2.042(4) 2_655 ?
O5A Fe2A 2.032(4) 4_565 ?
O5B Fe2B 1.950(4) 3_665 ?
O5C Fe2C 1.941(4) 4_566 ?
O5D Fe2D 2.001(4) 4_566 ?
O7D O7E 1.456(10) . ?
O9A B33 1.259(9) 2_655 ?
O10A B32 1.343(6) 4_565 ?
O10B B31 1.393(7) 3_665 ?
O10C B34 1.426(10) 4_566 ?
O10D B24 1.562(9) 4_565 ?
OW1A OW1B 1.176(10) . ?
